Arabian Journal of Chemistry (2011) 4, 235–237
King Saud University
Arabian Journal of Chemistry www.ksu.edu.sa www.sciencedirect.com
New route for preparation and characterization of magnetite nanoparticles M.A. Abdalla a, M.H. Jaafar a b
, Z.A. Al-Othman a, S.M. Alfadul b, M. Ali Khan
Department of Chemistry, College of Science, King Saud University, Riyadh, Saudi Arabia King Abdalaziz City for Science and Technology, Riyadh, Saudi Arabia
Received 29 June 2010; accepted 29 June 2010 Available online 3 July 2010
KEYWORDS Magnetite; Nanoparticles; Co-preparation; Characterization; Iron(II) chloride; Iron(III) chloride
Abstract We report here the synthesis of naked magnetic nanoparticles by using a facile method. Magnetic nanoparticles were prepared by mixing and stirring two equivalents of iron(II) chloride tetrahydrate with three equivalents of iron(III) chloride hexahydrate at room temperature. The mixture was treated by adding 100 ml of 28% ammonium hydroxide. Immediately, the color of the solution turned from orange to black. Magnetite nanoparticles precipitated and were washed three times with 5% NH4OH solution using the magnetic decantation method. pH¼9
2FeðIIÞ þ 3FeðIIIÞ ! Fe3 O4 # NH4 OH
The nanoparticles have been underwent full characterization. Their surface show a bunch of hydroxyl groups which they can be used for further complexion and removal of many hazardous compound. ª 2010 King Saud University. Production and hosting by Elsevier B.V. All rights reserved.
1. Introduction Nanoscale magnetite particles have drawn increasing interests in studying their application in environmental studies. There * Corresponding author. Tel.: +966 4675970. E-mail address: [email protected]
(M.H. Jaafar). 1878-5352 ª 2010 King Saud University. Production and hosting by Elsevier B.V. All rights reserved. Peer review under responsibility of King Saud University. doi:10.1016/j.arabjc.2010.06.061
Production and hosting by Elsevier
are different methods in the literature used for their synthesis with desired size, structure and other surface properties are described (Cornell and Schwertmann, 1996; Thuman, 1985; Trauth and Xanthopoulos, 1997; Solomons and Fryhle, 2004; Potter and Simmons, 1998; Readman et al., 2002; Anderson et al., 1980). These properties directly inﬂuence their chemical behavior of these nanoparticles and hence affect their application in different environmental application (Squillace et al., 1999; LaGrega et al., 2001; Rittman, 1987). Nanoscale magnetite particles being a nanoscale material with typical size range of 1–100 nm. Recent articles in the literature have shown that many of these particles properties depend on their size which is in nanoscale size. Beside it shows that coercive force in magnetic material can be changed with the enhancement of their mechanical strength. It is also affect their surface chemistry (Rittman, 1987; Lagwaldt and Puhakka, 2000; Grady, 1986).
M.A. Abdalla et al.
There are vast environmental application of this nanobased material particularly in cleaning up contaminated soil and ground water. Because these particles have smaller size this nanoscale magnetic iron materials are much more reactive than the conventional iron powders. Moreover they can be suspended in slurry and pumped straight to the contaminated site. Elemental metal iron is known to be non-toxic, and when oxidized in present of organic contaminants, these organic can be broken down into simple carbon compounds that are less toxic. It also known that oxidizing iron can reduce heavy metals to an insoluble form that tends to stay locked in soil. In this paper the magnetic ﬂuid containing Fe3O4 nanoparticles was prepared by the chemical co-precipitation of ferric and ferrous salts in alkaline medium using Reimer’s procedure (Balba et al., 2002; Hou et al., 2003; Al-Khamis et al., 2009). X-Ray Defraction.
2. Experimental 2.1. Chemicals and apparatus All chemicals used in experiment were of analytical grade. Iron(II) chloride tetrahydrated (99%) and iron(III) chloride hexahydrated (97%), ammonium hydroxide (28%) NH3 in double distilled water, are all from (BDH). FT-IR spectra were recorded by prestige -21-FT-IR spectrophotometer (Shimadzo). SEM spectra were recorded by JSM-6380LA scanning electron X-ray diffraction spectra were recorded by microscope (Jeol) Altima 4 X-ray diffraction (Rigaco). 2.2. Procedure To prepare Fe3O4 particles add two equivalent of FeCl2Æ4H2O to three equivalent of FeCl3Æ6H2O in 500 ml beaker and add 100 ml of double distilled water and stir the solution
SEM of Fe3O4 nanoparticles.
80 %T 70
New route for preparation and characterization of magnetite nanoparticles
Magnetic properties of Fe3O4 nanoparticles.
continuously at room temperature till complete dissolution is achieved. Then add 200 ml of ammonium hydroxide and allow the reaction to occur for around 15 min. The resulting particles were then washed three times with 5% ammonium solution. The precipitates were then ﬁltered and allowed to dry in air. The dried particles were then grounded in a mortar and then were examined with FT-IR, scanning electron microscopy, X-ray diffraction and PPMS (quantum design) measurements to investigate the crystal structure of the particles and magnetization of the sample material.
We conclude from that the efﬁciency and simplicity of the chemical co-precipitation method for the preparation of nanoscale magnetite with a super para-magnetism from the solution of iron(II)/iron(III)mixed salt-solution in aqueous ammonium hydroxide solution. The results show that Fe3O4 nanoparticles can be prepared in the sizes range from 10 to 20 nm. The use of these nanoscale particles in puriﬁcation of water from organic contaminant is under taken and is going to be reported later. As mentioned previously Fe3O4 nanoparticles which were prepared by the previous method can of course be promising as potentiality good magnetic material that can have good magnetic quality.
3. Results and discussion Acknowledgement Nanoscale magnetic particles were prepared by the chemical co-precipitation of iron(III) and iron(II) chloride salt in alkaline medium using Reimer’s procedure with slight modiﬁcation. Spectral characterizations have proven the formation of super magnetite nanocrystals of Fe3O4. In Fig. 1 the peak at 576.72 cm1 is attributed to the vibration of Fe–O band of Fe3O4, the peak at 1402 cm1 is assigned the Fe–O stretch of the Td. entity and the peak at 3134.33 cm1 is attributed to the stretching vibration of –OH which is assigned to OH adsorbed by Fe3O4 nanoparticles. Fig. 2 shows X-ray diffraction pattern of the Fe3O4 nanoparticles. The three main-peaks indicates that the nanoscale magnetite particles can be identiﬁed as Fe3O4. The X-ray spectra doses not show any other crystalline phases. The use of the X-ray also gave an indication of the crystallite size of Fe3O4 nanoparticles to be approximately 10 nm. Fig. 3 illustrates the SEM micrograph of the nanoscales magnetite particles. Morphology of the particles was uniform and each particle was approximately ranging between 10 and 70 nm in diameter. Fig. 4 presents the magnetization of Fe3O4 nanoparticles in a ﬁeld of 90 Oe on a super conducting quantum interference device magnetometer. The absent of a well-deﬁned maximum in the ZFC curve indicates that Fe3O4 nanoparticles exhibit blocking temperature above room temperature. It is known that the maximum of the ZFC curve for a collection of super paramagnetic non-interaction single-domain nanoparticles is dependent on the size of nanocrystals and their degree of clustering, as well as on the mutual dipolar interaction between them.
The authors would like to thank the Research Center, College of Science for ﬁnancial support (Project No. (Chem/2009/56). References Al-Khamis, Kh.M., Mahfouz, Refaat M., Abdulrahman, Al-Warthan A., Raﬁg-Siddiqui, M., 2009. Arabian J. Chem. 2, 73–77. Anderson, N., Bolto, B., Eldridge, R., Kolarik, O., Swinton, E., 1980. Water Res. 14 (8), 967–973. Balba, M., Blickle, F., Coons, D., Lin, C., Napolitan, M.R., Weston, A., 2002. In: Proceedings of the International Conference on Remediation of Chlorination and Recalcitrant Compounds, Third, Monterey, CA, United States, May 20–23, 2002, pp. 1013–1018. Cornell, R.M., Schwertmann, U., 1996. The Iron Oxides: Structure, Properties, Reactions. Occurrence and Uses. VCH, NY. Grady, C., 1986. Hazard. Waste Hazard. Mater. 3 (4), 333–365. Hou, Y., Yu, J., Gao, S., 2003. J. Mater. Chem. 13, 1983. LaGrega, M., Buckingham, P., Evans, J., 2001. The Environmental Resources Management Group. Hazardous Waste Management. McGraw-Hill Inc., New York, NY. Lagwaldt, J., Puhakka, J., 2000. Environ. Pollut. 107 (2), 187–197. Potter, T., Simmons, K., 1998. In: [email protected]
of Petroleum Mixtures, vol. 2. Amherst Scientiﬁc Amherst, MA. Readman, J., Fillmann, G., Tolosa, I., Bartocci, J., Villeneuve, J., Catinni, C., Mee, L., 2002. Mar. Pollut. Bull. 44 (1), 48–62. Rittman, B., 1987. Environ. Sci. Technol. 21 (2), 128–136. Solomons, T., Fryhle, C., 2004. Organic Chemistry, eighth ed. John Wiley and Sons Inc., New York. Squillace, P., Moran, M., Lapham, W., Price, C., Clawges, R., Zogor, J., 1999. Environ. Sci. Technol. 33, 4176–4187. Thuman, E., 1985. Organic Geochemical of Natural Water. Martinus nijhoff-Dr Junk, Dordrecht. Trauth, R., Xanthopoulos, C., 1997. Water Res. 31 (11), 2711–2718.